# A user-material subroutine incorporating single crystal plasticity in

date post

08-Dec-2016Category

## Documents

view

229download

2

Embed Size (px)

### Transcript of A user-material subroutine incorporating single crystal plasticity in

....

.. ~ -. MEClHI .. 178

A USER-MATERIAL SUBROUTINE INCORPORATING SINGLE CRYSTAL PLASTICITY

IN THE ABAQUS FINITE ELEMENT PROGRAM

Yonggang Huang

Division of Applied Sciences Harvard University

Cambridge, Massachusetts 02138

June 1991

A USER-MATERIAL SUBROUTINE

INCORPORATING SINGLE CRYSTAL PLASTICITY

IN THE ABAQUS FINITE ELEMENT PROORAM

Yonggang Huang

Division of Applied Sciences

Harvard University Cambridge, MA 02138

June 1991

Abstract

A user-material subroutine has been written to incorporate single crystal plasticity in the fmite element program ABAQUS. The fmite-element formulation of elastic-plastic and viscoplastic single crystal deformation is reviewed in this paper. including versions for small deformation theory and for the rigorous theory of finite-strain and fmite-rotation. Inelastic deformation of a single crystal arises from crystalline slip, which is assumed here to obey the Schmid law. Various

self and latent hardening relations between resolved shear stress and shear strain in slip systems are presented and incorporated as options in the subroutine.

1

1. Introduction

The finite element program ABAQUS has been widely used in the deformation and stress

analysis of solids. Besides a broad range of constitutive models, ABAQUS also provides an

interface whereby the user may write his or her own constitutive model in a subroutine denoted

UMAT in a very general way (ABAQUS User's Manual, 1989). The stresses, strains and solution

dependent state variables are solved incrementally by ABAQUS. When the subroutine UMAT is

called, it is provided with the state at the start of the increment (stress, solution dependent state

variables) and with the strain increments and the time increment The subroutine UMAT performs two functions: it updates the stresses and the solution dependent state variables to their values at the

end of the increment, and it provides the material Jacobian matrix, d~(J I dAE, for the constitutive

model as required for an iterative Newton-Rbapson solution.

The main objective of this paper is to provide the fmite element code ABAQUS a user-

material subroutine for the constitutive relation of single crystals in a continuum framework. The

kinematical structure here falls within the framework laid out by Rice (1971) and Hill and Rice

(1972), rigorously accommodating [mite deformation effects. The plastic deformation is assumed

due solely to the crystallographic dislocation slip; deformation by diffusion, twinning and grain

boundary sliding is not considered here. The Schmid stress, or resolved shear stress on a slip

system, is assumed here to be the driving force for slip. The completion of this subroutine makes

it possible to use ABAQUS for stress and fracture analyses of single crystals andbicrystals. The

- finite element analysis of single crystals was fust studied by Peirce, Asaro and Needleman (1982.

1983).

2. Review of Elastic-Plastic Constitutive Formulation for Single Crystals

2.1 Kinematics The Idnematical theory for the mechanics of crystals outlined here follows the pioneering

work of Taylor (1938) and its precise mathematical theory by Hill (1966), Rice (1971), and Hill

and Rice (1972). The following is a simple summary of the theory, followed Asaro and Rice

(1977) and Asar~ (1983).

A crystalline material is embedded on its lattice which undergoes elastic deformation and

rotation. The inelastic deformation of a single crystal is assumed here to arise solely from

crystalline slip. The material flows through the crystal lattice via dislocation motion. The total

defonnation gradient F is given by (2.1.1)

2

- ....

where FP denotes plastic shear of the material to an intennediate reference configuration in which

lattice orientation and spacing are the same as in the original reference configuration, and where F*

denotes stretching and rotation of the lattice. Elastic properties are assumed to be unaffected by

slip, in the sense that stress is detennined solely by F. The rate of change of FP is related to the

slipping rate y(a) of the a slip system by FP . FP- 1 = I y(a)s(a)m(a) (2.1. 1a)

a

where the sum ranges over all activated slip systems, unit vectors s(a) and m(a) are the Slip

direction and nonnal to slip plane in the reference configuration, respectively. It is convenient to define the vector s(a), lying along.the slip direction of system a in the

/

defonned configuration, by (2.1.2a)

A nonnal to the slip plane which is the reciprocal base vector to all such vectors in the slip pl~e is _ m(a)=m(a)F -1 (2.1.2b)

The velocity gradient in the cunent state is L=FF-1 =D+O (2.1.3)

where the symmetric rate of stretching D and the antisymmetric spin tensor Q may be decomposed

into lattice parts (superscript .) and plastic parts (superscript p) as follows:

satisfying

2.2 Constitutive laws

D=D* +DP~ 0=0* +OP

D* +0* =F* _F*-I, DP +OP =l:y(a)s*(a)m*(a) a

(2.1.4)

(2.1.5)

Following Hill and Rice (1972), the existence of an elastic potential, Cl>::Cl>(F), assures that the relation between the symmeuic rate of stretching of the lattice, D*, and the Jaumann rate of

v Cauchy stress 0, 0 ,is given by

v* * o +O(I:D ) =L:D (2.2.1)

where I is the second order identical tensor, L is the tensor of e!astic moduli having the full set of v*

symmetries Lijkl=LjikJ=Lijlk=Lklij, the Jaumann rate 0 is the corotational stress rate on axes that rotate with the crystal lattice, which is related to the corotational stress rate on axes rotating with the

v material, 0, by

(2.2.2)

v . where 0'=0-0'0+00.

3

The crystalline slip is assumed here to obey Schmid's law, i.e. the slipping rate yea) in any

particular slip system a is assumed to depend on the current 0' solely through the so-called Schmid

stress, t

where hap are the slip hardening moduli, the sum ranges over all activated slip systems. Here baa (no sum)"and bali (a:F~) are called self and latent hardening moduli, respectively.

Peirce, Asaro and Needleman (1982), and Asaro (1983a, b) have used a simple form for

the self hardening moduli:

haa = hey) = hoseCh2~ (no sum on a) ~

(2.3.3a)

where ho is the initial hardening modulus, to is the yield stress which equals the initial value of current strength g(a)(o), 't, is the stage I stress (or the break-through stress where large plastic flow

initiates), and y is the Taylor cumulative shear strain on all slip systems, i.e. I

y = l:J~(a)~t ao

(2.3.3b)

The latent hardening moduli are given by hap = qh(y) (a ~) (2.3.3c)

where q is a constant. These expressions of hardening moduli neglect the Bauschinger effect in a /

crystalline solid.

Bassani and Wu (1991) have used a different expression for the hardening moduli to

describe the three stage hardening of crystalline materials. Their expression depends on the shear

strains i a) of all slip systems:

baa = { (ho - b, )sech2[ (ho ~~ ~,~:

(-s(a),m(a as separate slip systems on each of which only positive slip is alJowed. Thus, we

pennit yea) to be negative if the corresponding t

!J:y(a) = ~t y(a) + a_v J_~'t(a) + a_v J_~g(a) [

~(a) :l,.V(a)] t ot(a) og(a) (3.1.4)

3.2 Incremental EOODulation

The relations are derived in this section for the increments of shear strain ~y..a), resolved

shear stress ~'t(a), current strength ~g(a) in all slip systems, in terms of the strain increments M1j v

and time increment ~L The corotational stress increments ~aij = aij ~t are also expressed in terms

of strain increments.M;} This definition of stress increment is consistent with the fmite element

code ABAQUS (ABAQUS theory manual, 1989; also Hughes and Winget, 1980) for Imite

deformation analysis.

It is convenient to introduce for each slip system the "Schmid factor" Jl~t) and tensor CI)~a)

defined as II~~) = .!.[s~(a)m~(a) +s~(a)m~(a)] "'IJ 2 I J J I

Ca) _ 1 [*(a) *(a) *(a) *(a)] Olij . - 2 Si mj -Sj mi

The tensor c.o~j) is related to the spin tensors a and 0* by n .. - rt = ~ c.o~~)y. (a)

lJ lJ "IJ a

(3.2.1a)

(3.2.lb)

(3.2.lc)

From the general hardening equation of crystalline slip (2.3.2), the increments of current

hardening function ~g(a) are given by (3.2.2)

The increments of resolved shear stress ~

(3.2.S) .

where 8a~ is the Kronecker delta. Once the Ilia) are known in tenns of the strain increments

~j, all other increments can be found through eqs. (3.2.2)-(3.2.4).

3.3 Lattice Rotation

The crystal lattice undergoes distortion and rotation as the crystal defonns; however, the

effect of lattice rotation does not explicitly appear in the constitutive equations in Section 2 when all

rate quantities are fonned on this rotating lattice frame. in slip systems is replaced by the following nonlinear equation.

8

--

which is obtained by substituting the general expression of the slipping rates (2.3.1) into the

incremental equation (3.1.2).

l1y(a> _ (1- 9)Arr(a) _ 9Aui(a)f(a>( t~a) + ~t(a) = 0 t g~a> + l1g(a) (3.4.1)

where the increments of resolved shear stress ~t(a) and current strengths ~g(a) are nonlinear

functions of ~"fa) determined by eqs. (3.2.2) and (3.2.3). The above nonli

*View more*